# Thermally-induced deformation behavior of unsymmetric laminates

Post on 02-Jul-2016

219 views

Embed Size (px)

TRANSCRIPT

<ul><li><p>Pergmon </p><p>lnt..L Solids Structures Vol. 35, No. 17, pp. 2101-2120, 1998 1998 Elsevier Science Ltd </p><p>All fights reserved. Printed in Great Britain 0020-7683/98 $19.00 + .00 </p><p>PII : S0020-7683(97)00167--4 </p><p>THERMALLY-INDUCED DEFORMATION BEHAVIOR OF UNSYMMETRIC LAMINATES </p><p>MARIE-LAURE DANO and MICHAEL W. HYER Department of Engineering Science and Mechanics, Virginia Polytechnic Institute and State </p><p>University, Blacksburg, VA 24061-0219, U.S.A. E-mail : hyerm@vt.edu </p><p>(Received 29 September 1996; in revised form 30 May 1997) </p><p>Abstraet--A methodology is presented to predict the displacements, particularly the out-of-plane component, of fiat unsymmetric epoxy-matrix composite laminates as they are cooled from their elevated cure temperature. Approximations to the grain fields are used in the expression for the total potential energy and the Rayleigh-Ritz technique is applied. Curvatures of the originally flat laminate as a function of temperature are predicted, as are the shapes of the laminates at room temperature. As geometrically nonlinear effects occur, stability is studied. As such, stability and the existence of multiple solutions, which are interpreted as multiple shapes, are prominent features of the problem. Experimental results are presented which confirm the predictions of the theory regard- ing the existence of multiple solutions, and the magnitude of the displacements. Results are compared with those of several other investigators, and limited finite element analyses are used to further study the problem. 1998 Elsevier Science Ltd. </p><p>BACKGROUND </p><p>When cured fiat in a press or autoclave, unsymmetric epoxy-matrix composite laminates will develop curvature when cooled to room temperature. The curvatures are due to a mismatch in the thermal expansion behavior of the layers within the laminate. A number of papers have been published which discuss the behavior. Hyer (1981a) investigated the shapes of several families of unsymmetric laminates and observed that the room- temperature shapes do not always conform to the predictions of classical lamination theory. Instead of being a saddle shape, as predicted by the classical theory [see, for example, Jones (1975)], many unsymmetric laminates have a cylindrical shape at room temperature. In addition, a second cylindrical shape can sometimes be obtained by a simple snap-through action. Hyer felt that incorporating geometric nonlinearities into the classical theory was necessary to explain this behavior. To correctly predict the room temperature shapes of cross-ply laminates, Hyer (1981b, 1982) and Hamamoto and Hyer (1987) developed a nonlinear theory based on polynomial approximations to the displacements, extended classical lamination theory to include geometric nonlinearities, and used a Rayleigh-Ritz minimization of total potential energy. In the theory inplane shear strain was assumed to be negligible. Jun and Hong (1990) modified Hyer's theory by including more terms in the polynomials to account for inplane shear strain. They found that shear strain was indeed negligible for square laminates with very large or small length-to-thickness ratios. However, for intermediate length-to-thickness ratios, shear strain can be significant. Recently, Schlecht et al. (1995) performed finite element analyses to calculate the room temperature shapes of square unsymmetric cross-ply laminates. The finite element analysis calculations compared very well with the predictions from Hyer's theory. </p><p>The various investigations demonstrate that the deformation behavior of unsymmetric laminates with cross-ply lay-ups is now well understood. The behavior of unsymmetric laminates with arbitrary lay-ups, however, is still not fully understood, though there has been work in this area. Dang and Tang (1986) modified Hyer's theory to predict the room temperature shapes of more general unsymmetric laminates. They generalized Hyer's theory by introducing more sophisticated polynomial displacement functions. Approximations of the displacements in the principal curvature coordinate system were used as a startitlg point. Through coordinate transformation, the displacements in the structural coordinate </p><p>2101 </p></li><li><p>2102 M.-L Dano and M. W. Hyer </p><p>system were computed. The distinction between the two coordinate systems used for the computation of the displacements is illustrated in Fig. 1, the structural coordinates having the x- and y-axes aligned with the edges of the laminate. Geometric nonlinearities were considered and a Rayleigh-Ritz approach based on the total potential energy was used to compute shapes. The assumed displacements were not specified correctly and only the sum of two coefficients in the assumed displacement functions could be solved for, as opposed to solving for each coefficient separately. Nonetheless, the comparisons with limited experimental data from Hyer (1981a) were good. </p><p>Adopting the same approach, several investigators have proposed different versions of the Dang and Tang theory. Jun and Hong (1992) modified Dang and Tang's approximate displacement functions by adding more polynomial terms. They obtained fairly complex generalized displacement expressions and used several changes of variables and trigono- metric relations to simplify these expressions. The modifications brought to Dang and Tang's theory appeared to affect the shapes for small length-to-thickness ratios. For larger length-to-thickness ratios, the differences were negligible. To validate the theory, a few experimental results for the principal curvature direction from Hyer (1981 a) were presented. No experimental results were presented for the magnitudes of the principal curvatures. Recently, Peeters et al. (1996) developed a theory for square angle-ply laminates based on the work of Jun and Hong (1992). They modified the displacement functions of Jun and Hong by using a more complete set of third-order polynomials. To compute the total potential energy, Peeters et al. fixed the value for the principal curvature direction, in Fig. 1, assuming it was 45 relative to the laminate edge for all laminates, as predicted by classical lamination theory. They arbitrarily forced the elongation strains in the principal curvature coordinate system to be independent of the coordinate variables in a certain fashion. They also treated the laminate as if it was square in the principal curvature coordinate system, the coordinate system which they assumed was oriented 45 relative to the edge of the square laminate! Experimental results from only a single + 30 angle-ply laminate were presented to compare with the theoretical model. The comparison between experiment and predictions was reasonable, but the authors went on to explain how manufacturing problems, material property uncertainties, and material inhomogeneities could have influenced their experimental results. The present paper will demonstrate that angle-ply laminates actually do not all have the same principal curvature direction. Rather, the principal curvature direction should be considered as a variable, and not be constrained a priori. </p><p>The theories developed so far to predict the shapes of general unsymmetric laminates follow the same approach used originally by Dang and Tang. This approach leads to expressions and procedures for obtaining the strains that seem to be unnecessarily complex. It was felt a theoretical model could be developed using a more straightforward approach </p><p>ii </p><p>x-y: Struomai (laminate) c, oordirmte system n-t: Principal curvature coordinate system ~: P r in~l curvature direction </p><p>Fig. 1. Principal curvature and structural coordinate systems. </p></li><li><p>Thermally-induced deformation behavior 2103 </p><p>and experiments could be conducted on a variety of laminates to compare with the model. These are the primary points of the present paper. </p><p>DEVELOPMENT OF THE THEORY </p><p>The theoretical model presented was developed to predict the deformation behavior of general unsymmetric laminates that are flat at their elevated curing temperature and are cooled to room temperature. It is based on a Rayleigh-Ritz minimization of the total potential energy. The key in using the Rayleigh-Ritz approach is to obtain good approxi- mations for the displacement functions to be used in the computation of the total potential energy. However, for the present problem these displacement functions are only used to obtain expressions for the strains needed to compute the laminate strain energy. There is no external work term in the total potential energy. Thus, instead of using approximations for the displacements, the present theory directly uses approximations for the laminate midplane strains, expressed in the laminate coordinate system. </p><p>Computation of the total potential energy Assuming a plane-stress formulation, the total potential energy of the laminate, H, </p><p>can be expressed as a function of the mechanical and geometrical properties of the laminate, the applied temperature change, AT, and the total strains by: </p><p>H fL;2 ILl2 fro2 (1 - 2 1 - 2 - = O,, ex + Q., 2e,~ey + Q., 6Y~yex + ~ Q22ey + Q26%,yey </p><p>O - rx/2 .I - Ly/2 d-H~2 </p><p>l 2 - "JC ~ 066~xy - - (Q l l ~x + ~_.~ 20~y "1- O l 6(Xxy)F'x AT- (Q12~ + 0220Cy -~- 0260~xy)ey AT </p><p>-- (~6~ + Q26~t e + 066~txy)y~y AT~ dxdy dz / </p><p>(1) </p><p>where Lx, Ly, and H are the length of the laminate in the x- and y-directions, and its thickness. The {jq's are the transformed reduced stiffnesses of the individual layers [see Jones (1975)] and the total strains e~, ey, y~y are given by </p><p>0 0 0 0 0 0 gx = ~'x "q- ZK'x gy = gy "JI- Zl(Jy ~: xy = ~'xy + zxxy. (2) </p><p>o 0 The quantities e , e , yoy and ~Cx , Xy, xxy are the laminate midplane strains and curvatures, respectively, defined by </p><p>o duO l( wO 2 = + ) </p><p>o Ov l (dw~ 2 o du Ov Ow dw ey=~y+~\~y j yxy = -~-y + ~-x + ~---~- -~-y (3) </p><p>02w 0 02w 0 02w 0 xo = __ __ 0 __ __ o -- 2 - - (4) </p><p>ax E ~; = OY 2 Xxy = Ox Oy </p><p>where it is seen that geometric nonlinearities in the sense of von Karman are included, and where u , v and w are the midplane displacements of the laminate in the x, y and z- coordinate directions. Here the extensional midplane strains are approximated using the following set of complete polynomials : </p><p>e = Coo + cl oX + Co t y + c2ox 2 + Cl i xy dl- Co2Y 2 + C3O x3 + C21 x2y + Cl 2xy 2 + Co3y 3 </p><p>e = doo+d~ox+doly+d2ox2+d, ,xy+do2y2+d3ox3+d21x2y+d,2xy2+do3y 3 (5) </p><p>where the cs and ds are to-be-determined coefficients. The particular functional forms for ~o and ~o are motivated by the desire to remain flexible as regard any assumed evenness or </p></li><li><p>2104 M.-L. Dano and M. W. Hyer </p><p>oddness of these strains with respect to the coordinate directions. The inplane shear strain is more difficult to assume, as it must be consistent with the strains s and +o. To assure consistent strains, the inplane shear strain is determined using strain--displacement relations. Based on past observations of a large number of unsymmetric laminates, the out-of-plane displacement, w , can be approximated by </p><p>w(x,y) = (ax 2 +byZ+cxy) (6) </p><p>where a, b and c are to-be-determined coefficients which represent, respectively, the negative of the curvatures in the x- and y-directions and the negative of the twist curvature, as </p><p>t~ 2 w 0 2 w o 0 2 w o _ o - b o 20 x o =-a x , .= x,,y . . . . c (7) </p><p>x:, = ax 2 " t3y2 t3y </p><p>and where it is seen that the curvatures are assumed to be a constant throughout the laminate. Alternatively, the curvatures a, b and c can be thought of as average curvatures. </p><p>Using the expressions for the extensional strains e and e , and the out-of-plane displacement w , the inplane displacements u and v can be determined by integrating the rearranged strain-displacement relations given by </p><p>Ou o 1 (Ow~ 2 0/3 0 o 1 (owO~ 2 0~- = ex - ~ k-~--x ] ay - ey- ~ k dy// " (8) </p><p>The two unknown functions of integration introduced by integrating eqn (8) to obtain u(x, y) and v(x, y) are assumed to be polynomials. The polynomials are chosen to make u(x, y) and v(x, y) complete polynomials to order three, and to suppress rigid body rotation about the z-axis. These steps result in five additional unknown coefficient, denoted ei, i = 1, 5. The inplane shear strain can then be easily computed by the third strain-displacement relation, namely, </p><p>Ou o &o Ow o Ow o ?,o . . . . </p><p>Oy + ~x + Ox Oy </p><p>= 2el +(e2+co l )x+(e4+dlo)y+ ab- ~ +2Co2+2d2o xy </p><p>+(~(2+C~l )+e3)x2+- (~(b- -~+d~)+es)Y 2 </p><p>c2 l 3 d12 3 +(3c03 +d21)xy 2 + (3d30 +c12)x2y+ -5 -x + --~-y (9) </p><p>This procedure ensures a consistent set of expressions for the needed midplane strains. None of the recent investigators studying more general unsymmetric laminates appeared to have taken this simple approach. The approximations obtained for the midplane strains use a total of 28 to-be-determined coefficients. </p><p>Back-substituting the midplane strains and curvatures into the total strains, eqn (2), and into the definition of the total potential energy, eqn (1), the spatial integrations in the expression for the total potential energy can be conveniently carried out. The final result is an algebraic expression for the total potential energy of the laminate of the form </p><p>[ l= l - I (AT , a,b,c, coo,Clo, Col,C2o,Cll,Co2,C3o,C21,c12,Co3, </p><p>doo,d~o,dol,d2o,dlL,doz,d3o,d2t,dl2,do3,ei) i=- 1,5. (10) </p></li><li><p>Thermally-induced deformation behavior 2105 </p><p>Obviously, II is also a function of the laminate material properties and geometry, but here interest centers on the unknown coefficients and the temperature change. </p><p>Minimization of the total potential energy To study the deformation of the laminate as it is cooled from its cure temperature, </p><p>AT < 0, the variation of the total potential energy is used. This is most conveniently done by allowing variations of the 28 displacement coefficients in eqn (10). Equating the first variation to zero results in 28 equilibrium equations for the laminate. Reorganizing the equations by eliminating some coefficients between them, the set of 28 equations can be reduced to a set of three nonlinear algebraic equations, which are functions of the curvatures a, b, c and the temperature change AT, and are of the form </p><p>f~(a,b,c, AT) = 0 fb(a,b,e, AT) = 0 f . (a ,b ,e ,AD = O. (11) </p><p>Solving these equations as a function of AT using the Newton-Raphson technique gives the configuration of the laminate as it cools from the flat curing stage. The above set of nonlinear algebraic equations admits multiple solutions, each solution corresponding to a different configuration, i.e. different bending and twist curvatures a, b and c. The stability of the configurations can be assessed by examining the higher-order variations of the total potential energy, or the Jacobian offa, fb andf~ needed in the Newton-Raphson technique. Here the latter approach was used. This is all accomplished with the aid of the sym- bolic manipulation package Mathematica [see Wolfram (1991)] and specifically-written FORTRAN programs. </p><p>NUMERICAL RESULTS </p><p>The set of three equations given by eqn (11)...</p></li></ul>